^{1}

^{1}

^{2}

Beryllium aluminum cyclosilicate, an ore of beryllium was reinforced in Aluminum matrix to fabricate Al-beryl composites using powder metallurgy. Effect of the content of beryllium aluminum cyclosilicate on microstructural hardness and thermal expansion was studied. The coefficient of thermal expansion of Al-beryl composite was measured in the temperature range between 50
^{o}C to 360
^{o}C using dilatometer and was theoretically studied using thermo-elastic models, and these models were used to explain abnormalities observed experimentally. The hardness of Al-beryl metal matrix composites increased with the increase in beryl percentage. Vacuum sintering of Al-beryl metal matrix composites at 600
^{o}C inhibited excellent bonding between the matrix and the particulate increasing the strength of the composite. The result shows the CTE significantly increased with increasing temperature but decreased with increasing reinforcement. At higher temperatures, CTE of Al-beryl metal matrix composites with 5 wt%, 10 wt% and 15 wt% of beryllium aluminum cyclosilicate was 21 ppm/K, 18.2 ppm/K, and 16.8 ppm/K. The CTE values were found to be comparable with theoretical results. The turner model showed conformance with experimental results, was well suited to the experimental results.

Metal matrix composites (MMCs) have been undergoing various technological advances and emerged as a class of materials suitable for structural, thermal and wear applications. They exhibit significant improvement in physical and mechanical properties compared with monolithic materials in strength, elastic modulus, fatigue resistance and tribological properties at room and elevated temperatures [

The coefficient of linear thermal expansion (CTE or α) is a material property that is indicative of the extent to which a material expands upon heating [

There are three several types of coefficients of thermal expansion: linear, superficial and volumetric CTEs. The measurement of the linear CTE is denoted by α and is given by

where, L_{0} is the original length of the sample, and

where,

where,

Many analytical models developed by Kerner, Turner, and Schapery bounds [

In the present study, an attempt was made to study linear CTE of Al-beryl MMCs and its effect on reinforcement percentage of beryl particles and temperature. The CTE of Al-beryl MMCs was measured between 30˚C and 350˚C by a high precision dilatometer, and the experimental results were compared with thermo-elastic models, and an appropriate model was proposed to predict CTE of Al-beryl MMCs.

First, commercially available pure aluminum, hereby referred as Al, was selected as a base metal. Al has a low density with good corrosion resistance, strength, ductility and improved tribological properties. The chemical composition of commercially available pure Al is given in

Beryl used as reinforcement, is a ceramic material for high-temperature applications because of its high melting point, lower density and capacity to retain high strength at elevated temperatures. Beryl with chemical formula Be_{3}Al_{2}Si_{6}O_{18 }with a hexagonal crystal structure is a naturally occurring ceramic particle. It has a specific gravity of 2.6 to 2.8 with a hardness of 7.5 to 8 on Mohs scale. Beryl does not have a sharp melting point but softens between temperatures 1475˚C and 1550˚C and has a low CTE of 2.6 × 10^{−6}/K [

The Beryl was procured in the form of stones and was crushed to powder form

Si | Fe | Al |
---|---|---|

0.14 | 0.16 | Balance |

SiO_{2} | Al_{2}O_{3} | BeO | Fe_{2}O_{3} | CaO | MgO | Na_{2}O | K_{2}O | MnO |
---|---|---|---|---|---|---|---|---|

65.41 | 17.94 | 12.3 | 0.8 | 1.34 | 0.48 | 0.55 | 0.004 | 0.05 |

using a ball mill. A proper ball to powder ratio was maintained to avoid powder agglomeration [

CTE is measured as per ASTM E228 standards using tube dilatometer (Model: BSPIL-MTR-DM). A dilatometer consists of an oven, support to hold the samples, thermocouples and LVDT sensors. Samples can be heated up to 1200˚C. The sample holder and push rod can accommodate samples up to 60 mm long. Temperature is recorded with K-type thermocouples located at the support for the measurement of sample temperature and at the center of the oven which is used to detect and control the heating temperature. The accuracy of CTE measured by this instrument is equal to ±0.1 × 10^{−6}/K.

Before A particulate composite is a homogeneous material having a uniform distribution of the particles in the matrix. Volume fractions of the two phases are V_{1} and V_{2}. The CTE of the MMCs is depended on several factors like matrix, size, and shape of the particles, distribution, type of particles and the microstructure of the composite. For the prediction of CTE of MMCs many models based on thermo-elastic energy principles were used such as Kerner, Schapery, and Turner models [

The following assumptions are made during the calculation of CTE using thermo-elastic models:

a) The bonding between Al matrix and the beryl particulates are perfect, and no chemical interactions are allowed between the matrix and the particle.

b) The properties of the constituents do not change with temperature.

c) Poisson’s ratios of the components are not very different.

The composites are isotropic and homogeneous. The Kerner model considers the particles as spherical in shape and discontinuous. CTE of a composite consisting of spherical particles dispersed in a matrix is given by

where

K is the bulk modulus of the of the composite, which is related to Young’s modulus E and the Poisson’s ratio m of isotropic materials by

Schapery bounds assume that the composite behaves as isotropic material and helps to determine CTE by considering the stress interaction between the matrix and the reinforcement. This model gives upper and lower bounds for the thermal expansion coefficient.

Upper bound is given by

Lower bound is given by

Turner model considers that internal stresses developed between the matrix and the reinforcement are not enough to disrupt the composite. The sum of the internal forces can be equated to zero, and an expression of the CTE of the composite is obtained as:

Turner model considers that there is a homogeneous strain throughout the composite, i.e., strain at every component in the composite changes in the same rate as a composite. Turner model assumes that uniform hydrostatic stresses exist in the phases and shear deformation is negligible.

Particle size influences processing conditions, microstructure, and properties of the composite. The size and shape of particles influences parameters like green strength, compressibility, apparent density, agglomeration, flow rate, porosity, and sinterability. Particle size analysis of beryl powders is carried out by laser diffraction technique using Mastersizer 2000, which confirms to ISO13320-1 guidelines. The results are shown in

μm and 38 μm.

Scanning electron microscope (SEM) images of Al powder (

Micrographs of the transverse section of Al-beryl MMCs are shown in

The Vickers hardness test was performed to determine themicro hardness of Al- beryl MMCs with a load of 100 g for the duration of 10 s as per ASTM E92 standards. The hardness is tested at three separate locations on the specimen, and the average of 3 readings was taken for a single specimen. The hardness of Al-beryl composites, by varying reinforcement content from 5% by wt. to 15% by wt. and the effect of sintering temperature and beryl particle size is presented in

The thermal expansion coefficients of Al-beryl MMCs with different weight

Beryl Reinforcement (wt%) | ||||
---|---|---|---|---|

Temperature (˚C) | 0 (10^{−6} K^{−1}) | 5% (10^{−6} K^{−1}) | 10% (10^{−6} K^{−1}) | 15% (10^{−6} K^{−1}) |

60 | 23.1 | 1.90 | 1.80 | 0.50 |

80 | 23.8 | 7.80 | 2.20 | 1.30 |

100 | 24.2 | 10.1 | 5.20 | 2.60 |

120 | 24.6 | 11.5 | 7.40 | 5.50 |

140 | 24.9 | 13.0 | 9.40 | 7.80 |

160 | 25.2 | 14.6 | 12.0 | 9.50 |

180 | 25.5 | 15.5 | 12.9 | 11.2 |

200 | 25.7 | 15.8 | 13.7 | 12.6 |

220 | 26.1 | 17.0 | 14.8 | 13.3 |

240 | 26.6 | 17.3 | 15.5 | 13.6 |

260 | 27.4 | 18.2 | 16.0 | 14.5 |

280 | 27.6 | 18.9 | 16.8 | 15.0 |

300 | 27.7 | 19.4 | 17.3 | 15.5 |

320 | 28.5 | 20.2 | 17.5 | 15.8 |

340 | 29.0 | 20.7 | 17.8 | 16.0 |

360 | 29.4 | 21.0 | 18.2 | 16.8 |

percentage of are shown in

Young’s modulus and CTE of pure aluminum and beryl at different temperatures are used to determine theoretical values of CTE using thermo-elastic models. Thermal expansion coefficients of Al-beryl MMCs obtained from dilatometry are plotted together with the values obtained from thermo-elastic models given in the previous section, as shown in

Al-beryl MMCs with 5% to 15% by weight percentage of beryl were successfully fabricated using powder metallurgy process. The following conclusions can be drawn from this study.

・ The thermal expansion coefficients of Al-beryl MMCs decrease with the increase in beryl content between the temperature ranges 0˚C to 360˚C. Further, the CTE values of Al-beryl MMCs remain uniform over a large temperature range which is an advantage.

・ Thermo-elastic models like Kerner model, Turner model, Schapery upper and lower bounds are used to evaluate and predict CTE of Al-beryl MMCs. The experimental values of thermal expansion of Al-beryl MMC are compared with thermo-elastic models, and the results fairly agree with those predicted by the Turner model at higher temperatures. Kerner model agrees with experimental values only at lower reinforcement percentages but overestimates the CTE values at 10% and 15% reinforcement of beryl by weight.

・ The discrepancy between the theoretical values and experimental values of the CTE could be due to the anisotropic nature of beryl with the different coefficients of expansion in various crystallographic directions and the lack of perfect bonding between the metal matrix and beryl particulates.

Bharat, V., Prasad, B.D. and Venkateswarlu, K. (2017) Effect of Beryllium Aluminum Cyclosilicate on Ther- mal Expansion Behavior of Al-Based Com- posites. Journal of Minerals and Materials Characterization and Engineering, 5, 140- 152. https://doi.org/10.4236/jmmce.2017.53012